(2) M. Calixto-Rodriguez et al. / Applied Surface Science 256 (2010) 2428–2433. 2. Experimental details 2.1. Deposition of thin ﬁlms Sb2S3 thin ﬁlms were prepared using the chemical bath deposition technique, following the procedure reported by Nair et al. . The bath was prepared using antimony trichloride (SbCl3) and sodium thiosulfate (Na2S2O3) as follows: In a 100 ml beaker, we have used 721 mg instead of 650 mg of SbCl3 which was dissolved in 2.5 ml of acetone. To this mixture was added 25 ml of sodium thiosulfate 1 M followed by 72.5 ml of deionized cold water (both maintained 10 8C) and stirred well. Borosilicate microscope glass slides from Corning with dimensions of 7.5 cm 2.5 cm 0.1 cm were used as substrates. The substrates were placed vertically in the solution. The deposition was made at 10 8C for 4 h without stirring. At the end of the deposition the slides, coated on both sides with orange yellow ﬁlms, were removed from the bath, washed well with distilled water, and dried with a constant ﬂow of air. The coating deposited on the side of the substrate facing the wall of the beaker was retained for nitrogen plasma treatments and thermal annealing in nitrogen atmosphere. The coating on the other side was wiped off with dilute acid. Thickness of the ﬁlms was measured using an Alpha Step model 100 proﬁlometer from Tencor Instruments. Typical thickness obtained for as-deposited ﬁlms was 385 nm, while for ﬁlms after nitrogen plasma treatment and thermal annealing in nitrogen atmosphere were 311 and 260 nm, respectively. 2.2. Post-deposition treatments of antimony sulﬁde thin ﬁlms The experimental apparatus and technique to generate the pulsed plasma was recently reported [19,20]. A brief description is reported here. The discharge chamber used in this work has two stainless steel circular plate electrodes, 1 mm thick and 30 mm in diameter. The electrodes are positioned horizontally at the center of the reaction chamber with 4 mm of separation between them. Samples were placed on the bottom electrode. The N2 gas was injected into the reaction chamber through the front ﬂange. The same gas connection was used for pressure sensor. The discharge power supply was maintained at an output of 300 V and a current of 0.36 A. The base pressure of the reaction chamber was maintained at 3.0 102 Torr using a mechanical pump (Varian SD-301) and purged with nitrogen at 1.0 Torr for several times in order to remove the background gases. The as-deposited antimony sulﬁde thin ﬁlms were treated with nitrogen plasma at 3.0 Torr during 60 min. For the as-deposited antimony sulﬁde thin ﬁlms, a thermal treatment in nitrogen atmosphere at 300 8C and 300 mTorr during 60 min was undertaken, which was performed in an oven with temperature and pressure controls. The as-deposited, plasma treated, and thermally annealed thin ﬁlms were structurally, compositionally, morphologically, optically and electrically characterized.. 2429. done using a Nanosurf EasyScan E-line equipment, the topography contrast images were acquired in the contact mode. For the optical emission spectroscopy (OES) analysis, an optic ﬁber was connected to the entrance aperture of a high-resolution Ocean Optics Inc. Spectrometer Model HR2000CG-UV-NIR, equipped with a 3 105 lines-ml composite blaze grating and a UV2/OFLV-5 detector (2048-element linear silicon CCD array). The grating response has a spectral response in the range of 200–1100 nm with efﬁciency >30%. The optical transmittance at normal incidence, and specular reﬂectance spectra of the samples were measured with a spectrophotometer Shimadzu model UV-1601PC in the UV–vis–NIR region (190–1100 nm wavelength range). For the electrical measurements, current versus time data were recorded on an automated system using a Keithley 619 electrometer and a Keithley 230 programmable voltage source. A pair of coplanar silver print electrodes of 3 mm in length, 3 mm in separation, was applied on the surface of the ﬁlms. 3. Results and discussion 3.1. X-ray diffraction (XRD) and compositional analyses Fig. 1 shows the X-ray diffraction (XRD) patterns for asdeposited, plasma treated, and thermally annealed antimony sulﬁde thin ﬁlms. No diffraction peaks were observed in the XRD pattern of the as-deposited thin ﬁlm, indicating that the deposited material is either amorphous or of poor crystallinity. It is a common result for as-prepared antimony sulﬁde thin ﬁlms obtained by the chemical bath deposition method [21–24]. The diffraction patterns corresponding to ﬁlms after nitrogen plasma treatment, and thermal annealing match well the standard for Sb2S3 (JCPDS 42-1393) which has an orthorhombic structure. The XRD pattern of the Sb2S3 thin ﬁlm after thermal annealing showed peaks higher than those obtained for ﬁlm treated with nitrogen plasma, with a preferential orientation along the (3 1 0) direction. The mean value of the crystallite sizes for the Sb2S3 thin ﬁlms treated with nitrogen plasma and ﬁlms thermally annealed were calculated for the diffraction peak oriented in the direction (3 1 0) using the Scherrer formula D = (0.9l)/(bcos u), where D is the diameter of crystallites, l is the wavelength of. 2.3. Characterization XRD diffraction patterns were recorded on a Rigaku D-Max Xray diffractometer using Cu-Ka radiation (l = 1.5406 A˚). The chemical composition of the as-deposited, plasma treated, and thermally annealed antimony sulﬁde thin ﬁlms was determined by energy dispersive X-ray spectroscopy (EDS) using an Inca Oxford Instruments system attached to the scanning electron microscope (SEM). The surface morphology was studied by scanning electron microscopy (SEM) JEOL model JSM 5800LV at 15 kV and 10,000. Atomic force microscopy (AFM) analysis was. Fig. 1. X-ray diffraction patterns for as-deposited, plasma treated, and thermally annealed antimony sulﬁde thin ﬁlms..
(3) M. Calixto-Rodriguez et al. / Applied Surface Science 256 (2010) 2428–2433. 2430. Table 1 Chemical composition of antimony sulﬁde thin ﬁlms by EDS. Sample. Sb (at%). S (at%). As-prepared Plasma treated Thermally treated. 46.54 45.50 46.70. 53.46 54.50 53.30. CuKa line, b is full width at half maximum (FWHM) in radians and u is Bragg’s angle. The mean crystallite size for the plasma treated ﬁlm was 13.7 nm, and for the ﬁlm thermally annealed was 19.1 nm. The nitrogen plasma and thermal treatments improved the crystalline structure of the as-deposited antimony sulﬁde thin ﬁlms. Table 1 shows the chemical composition in atomic percent (at%) for as-deposited, plasma treated, and thermally annealed antimony sulﬁde thin ﬁlms. The chemical composition on asdeposited ﬁlms was: 53.46% for S and 46.54% for Sb, this suggests that the as-deposited ﬁlms are close to the Sb2S3 stoichiometric composition. The decrease in the antimony content obtained for the ﬁlm after plasma treatment might be due to the plasma etching of this element on the surface of the ﬁlm. The little decrease in the sulfur content obtained for ﬁlm after thermal annealing is probably due to the loss of sulfur during the annealing process. 3.2. Morphological analysis Fig. 2 shows typical SEM pictures of the morphology of (a) asdeposited, (b) thermally annealed, and (c) plasma treated antimony sulﬁde thin ﬁlms. There are no signiﬁcant changes in the morphology for the as-deposited and plasma treated ﬁlms. The morphology in the thermally annealed ﬁlm looks very smooth. In the three cases there are clusters of quasi-spherical shape and varying size. The mean grain sizes of these clusters on the surface of the as-deposited, plasma treated, and thermally annealed ﬁlms are 249, 313, and 359 nm, respectively.. Fig. 3 shows typical AFM images of the surface topography in 3D for the antimony sulﬁde thin ﬁlms: (a) the as-deposited ﬁlm is formed by very small grains; (b) the thermally annealed ﬁlm shows that the small grains had coalesced because of the annealing temperature, resulting in a uniform surface with some additional big grains observed on the ﬁlm surface; and (c) for plasma treated ﬁlm, the surface is uniform and smoother than those observed in the other conditions. The root mean square (rms) value for asdeposited ﬁlm is 6.7 nm, meanwhile the rms values are modiﬁed for thermally annealed and plasma treated ﬁlms. The rms for thermally annealed ﬁlm was 8.1 nm, this increase in the roughness is induced by the cluster growth. The value of the roughness for the ﬁlm after plasma treatment was lower (6.0 nm) compared to that obtained for the as-deposited ﬁlm. This may be due to the erosion of the ﬁlm during the plasma process. 3.3. Optical emission spectroscopy (OES) analysis The interaction of the nitrogen plasma and the surface of antimony sulﬁde thin ﬁlm allows the generation of new species in the plasma. To identify these species, OES measurements were carried out during the experiments. Fig. 4 shows a typical optical emission spectrum for the plasma. The measurements allowed the analysis of the most luminous area that corresponds to the negative glow near the cathode dark space. The identiﬁed species from the Sb2S3 ﬁlm–nitrogen plasma interaction were: N2 at 235.14 nm (D3Su+-B3P g), 246.16 nm (A3Su+-X1Sg+), 280.46, 295.32, 297.68, 313.60, 315.93, 337.13, 353.67, 370.62, 380.49, 399.84, 405.94, and 434.36 (C3Pu-B3Pg); N2+ at 334.96, and 375.61 (B2Su+-X2Sg+); NS at 246.56 (A2D-X2P), 258.48 (A2DX2P), 258.70 (C2S-X2P), 269.74 (A2D-X2P), 419.17 (B2P-X2S); S2 at 269.76 (f1Du-a1Dg), 313.22, 355.56, 358.72, 393.89, 419.36, and 456.30 (B3Su-X3Sg); and SbS at 380.87, 399.18, 413.68, and 448.73 [25,26]. The majority of the species are vibrationally excited. S2 and SbS species were detected in the plasma, the origin of these species is from the ﬁlm surface, so plasma treatment changed the chemical composition of the Sb2S3 ﬁlm as revealed by the EDS analysis.. Fig. 2. SEM images for (a) as-deposited, (b) thermally annealed, and (c) plasma treated antimony sulﬁde thin ﬁlms..
(4) M. Calixto-Rodriguez et al. / Applied Surface Science 256 (2010) 2428–2433. 2431. Fig. 3. AFM images for (a) as-deposited, (b) thermally annealed, and (c) plasma treated antimony sulﬁde thin ﬁlms.. For allowed direct transitions, ahn is given by . 3.4. Optical and electrical properties Fig. 5a–c shows the behavior of the optical transmittance T(l) and specular reﬂectance R(l) spectra for as-deposited, plasma treated, and thermally annealed antimony sulﬁde thin ﬁlms. The as-prepared ﬁlms are transparent at wavelengths, l > 526 nm. A shift in the absorption edge toward larger wavelength is observed for plasma treated and thermally annealed ﬁlms. The values of the absorption coefﬁcient a(l) for the as-deposited, plasma treated, and thermally annealed ﬁlms were calculated from the data obtained from the transmission T, reﬂection R, and thickness d, using the well-known relationship  T¼. ð1 RÞ2 expðadÞ R2 expðadÞ. :. (1). Fig. 4. Typical OES spectrum for nitrogen plasma-Sb2S3 thin ﬁlm interaction.. 2. ðahnÞ ¼ Aðhn Eg Þ;. (2). where A is a constant and Eg is the optical band gap. Thus Eg can be obtained from a plot of (ahn)2 versus hn. The Eg values were calculated from the best ﬁt of the plot (ahn)2 versus hn, and its extrapolation to (ahn)2 = 0 (see Fig. 6). The as-deposited antimony sulﬁde thin ﬁlm has a band gap of 2.36 eV. The Eg values for plasma treated and thermally annealed Sb2S3 ﬁlms were 1.83 and 1.75 eV, respectively. A higher band gap for the as-deposited ﬁlm (2.36 eV versus 1.75 eV for thermally annealed ﬁlms) is attributed to size quantization as explained by Nair et al.  and Salem and Selim  for chemically deposited antimony sulﬁde thin ﬁlms. The reduction in the band gaps of the ﬁlms after post-deposition treatments is ascribed to the improvement in the crystallinity, which is evidenced in the XRD patterns given in Fig. 1. The electrical resistivity (r) value for the as-deposited thin ﬁlm was 6.2 108 V-cm. The r values for plasma treated and thermally annealed Sb2S3 thin ﬁlms were 4.5 106 and 5.3 108 V-cm, respectively. A r value of 108 V-cm was reported by Cardenas et al.  for chemically deposited antimony sulﬁde thin ﬁlms after annealing in nitrogen at 300 8C. Although, ﬁlms after thermal treatment had better crystalline structure compared to as-deposited ﬁlms, it was not observed a decrease in its electrical resistivity. Films after plasma treatment showed a reduction in the electrical resistivity in two orders of magnitude, this might be due to the etching at the ﬁlm surface. The etching at the ﬁlm surface in the plasma treatment improved the electrical transport at the surface. Note that the electrical measurements were done on the surface of the ﬁlms in the planar conﬁguration. It was unable to measure the conductivity type using the hot point probe technique in these samples because of its high electrical resistivity..
(5) 2432. M. Calixto-Rodriguez et al. / Applied Surface Science 256 (2010) 2428–2433. Fig. 5. T(l) and R(l) for as-deposited, thermally annealed, and plasma treated antimony sulﬁde thin ﬁlms.. Fig. 6. Plots of (ahn)2 versus hn for as-deposited, thermally annealed, and plasma treated antimony sulﬁde thin ﬁlms.. 4. Conclusions. Acknowledgements. Antimony sulﬁde thin ﬁlms chemically deposited were treated in nitrogen plasma and thermal annealing in nitrogen atmosphere to compare their structural, optical and electrical properties after the post-deposition treatments. XRD results revealed that the best crystallization of the ﬁlms was obtained by thermal annealing. The Eg values for plasma treated and thermally annealed antimony sulﬁde thin ﬁlms were 1.83 and 1.75 eV, respectively. Films after thermal annealing in nitrogen atmosphere did not show any change in the electrical resistivity value (108 V-cm). Films after plasma treatment showed a reduction in the electrical resistivity from 108 to 106 V-cm. Plasma treatments can be used to improve the electrical properties of as-deposited Sb2S3 thin ﬁlms.. The authors are thankful to Maria Luisa Ramo´n for the XRD measurements (CIE-UNAM), Jose´ Ortega (CIE-UNAM) and A. Gonza´lez (ICF-UNAM) for technical support, M.T.S. Nair and P.K. Nair (CIE-UNAM) for providing some experimental facilities, and M.E. Calixto for valuable discussions. One of the authors (MCR) acknowledges the ﬁnancial support received from DGAPA-UNAM. This research was partially sponsored by DGAPA IN-105707-3, DGAPA IN 111506, and CONACyT 41072-F. References  M.J. Chockalingam, K.N. Rao, N. Rangarajan, C.V. Suryanarayana, Studies on sintered photoconductive layers of antimony trisulphide, J. Phys. D: Appl. Phys. 3 (1970) 1641–1644..
(6) M. Calixto-Rodriguez et al. / Applied Surface Science 256 (2010) 2428–2433  E. Montrimas, A. Pazˇera, Charge carrier transport and space charge in thin ﬁlms of antimony trisulphide, Thin Solid Films 34 (1976) 65–68.  J. George, M.K. Radhakrishnan, Electrical conduction in coevaporated antimony trisulphide ﬁlms, Solid State Commun. 33 (1980) 987–989.  K.Y. Rajpure, C.H. Bhosale, (Photo)electrochemical investigations on spray deposited n-Sb2S3 thin ﬁlm/polyiodide/C photoelectrochemical solar cells, Mater. Chem. Phys. 63 (2000) 263–269.  Y. Rodrı´guez-Lazcano, M.T.S. Nair, P.K. Nair, Photovoltaic p-i-n structure of Sb2S3 and CuSbS2 absorber ﬁlms obtained via chemical bath deposition, J. Electrochem. Soc. 152 (2005) G635–G638.  K. Bindu, M.T.S. Jose´ Campos, A. Nair, P.K. Sa´nchez, Nair, Semiconducting AgSbSe2 thin ﬁlm and its application in a photovoltaic structure, Semicond. Sci. Technol. 20 (2005) 496–504.  K. Bindu, M.T.S. Nair, T.K. Das Roy, P.K. Nair, Chemically deposited photovoltaic structure using antimony sulﬁde and silver antimony selenide absorber ﬁlms, Electrochem. Solid-State Lett. 9 (2006) G195–G199.  S. Messina, M.T.S. Nair, P.K. Nair, Antimony sulﬁde thin ﬁlms in chemically deposited thin ﬁlm photovoltaic cells, Thin Solid Films 515 (2007) 5777–5782.  A. Arato, E. Ca´rdenas, S. Shaji, J.J. O’Brien, J. Liu, G. Alan Castillo, T.K. Das Roy, B. Krishnan, Sb2S3:C/CdS p-n junction by laser irradiation, Thin Solid Films 517 (2009) 2493–2496.  K. Bindu, M.T.S. Nair, P.K. Nair, Chemically deposited Se thin ﬁlms and their use as a planar source of selenium for the formation of metal selenide layers, J. Electrochem. Soc. 153 (2006) C526–C534.  R. Sagar, M.P. Srivastava, Amorphization of thin ﬁlm of CdS due to ion irradiation by dense plasma focus, Phys. Lett. A 183 (1993) 209–213.  Z.Y. Zhong, Y.D. Jiang, Surface modiﬁcation and characterization of indium-tin oxide for organic light-emitting devices, J. Colloid Interface Sci. 302 (2006) 613–619.  G. Lavareda, C. Nunes de Carvalho, A. Amaral, E. Fortunato, P. Vilarinho, a-Si:H TFT enhancement by plasma processing of the insulating/semiconductor interface, Mater. Sci. Eng. B 109 (2004) 264–268.  P. Arun, A.G. Vedeshwar, Laser induced crystallization in Sb2S3 ﬁlms, Mater. Res. Bull. 32 (1997) 907–913.. 2433.  R.K. Debnath, A.G. Fitzgerald, Electron beam induced surface modiﬁcation of amorphous Sb2S3 chalcogenide ﬁlms, Appl. Surf. Sci. 243 (2005) 148–150.  I. Grozdanov, A simple and low-cost technique for electroless deposition of chalcogenide thin ﬁlms, Semicond. Sci. Technol. 9 (1994) 1234–1241.  M.T.S. Nair, Y. Pen˜a, J. Campos, V.M. Garcia, P.K. Nair, Chemically deposited Sb2S3 and Sb2S3-CuS thin ﬁlms, J. Electrochem. Soc. 145 (1998) 2113–2120.  B. Krishnan, A. Arato, E. Cardenas, T.K. Das Roy, G.A. Castillo, On the structure, morphology, and optical properties of chemical bath deposited Sb2S3 thin ﬁlms, Appl. Surf. Sci. 254 (2008) 3200–3206.  M. Calixto-Rodriguez, H. Martı´nez, A. Sanchez-Juarez, AC plasma induced modiﬁcations in b-In2S3 thin ﬁlms prepared by spray pyrolysis, Thin Solid Films 517 (2009) 2332–2334.  H. Martı´nez, F.B. Yousif, Electrical and optical characterization of pulsed plasma of N2–H2, Eur. Phys. J. D 46 (2008) 493–498.  K.C. Mandal, A. Mondal, A new chemical method for preparing semiconductor grade antimony tri-sulphide thin ﬁlms, J. Phys. Chem. Solids 51 (1990) 1339– 1341.  O. Savadogo, K.C. Mandal, Studies on new chemically deposited photoconducting antimony trisulphide thin ﬁlms, Sol. Energy Mater. Sol. Cells 26 (1992) 117–136.  I. Grozdanov, A simple and low cost technique for electroless deposition of chalcogenide thin ﬁlms, Semicond. Sci. Technol. 9 (1994) 1234–1241.  C.D. Lokhande, B.R. Sankapal, R.S. Mane, H.M. Pathan, M. Muller, M. Giersig, V. Ganesan, XRD, SEM, AFM, HRTEM, EDAX and RBS studies of chemically deposited Sb2S3 and Sb2Se3 thin ﬁlms, Appl. Surf. Sci. 193 (2002) 1–10.  R.W.B. Pearse, A.G. Gaydon, The Identiﬁcation of Molecular Spectra, University Printing House Cambridge, Great Britain, 1976.  http://physics.nist.gov/PhysRefData/Handbook/element_name.htm.  T.S. Moss, Optical Properties of Semiconductors, Butterworths, London, 1959.  K.L. Chopra, S.R. Das, Thin Film Solar Cells, Plenum Press, New York, 1983.  A.M. Salem, M.S. Selim, Structure and optical properties of chemically deposited Sb2S3 thin ﬁlms, J. Phys. D: Appl. Phys. 34 (2001) 12–17.  E. Cardenas, A. Arato, E. Perez-Tijerina, T.K. DasRoy, G. AlanCastillo, B. Krishnan, Carbon-doped Sb2S3 thin ﬁlms: structural, optical and electrical properties, Sol. Energy Mater. Sol. Cells 93 (2009) 33–36..